Contents lists available atScienceDirect
Application of HVOF WC-Co-Cr coatings on the internal surface of small
ect of internal diameter on the wear resistance
, F. Venturia
, Z. Palab
, S. Kamnisc,**
, T. Hussaina,*
aFaculty of Engineering, University of Nottingham, Nottingham, NG7 2RD, UK bGE Aviation, Beranovych 65, Prague, Czech Republic
cCastolin Eutectic -Monitor Coatings Ltd, North Shields, NE29 8SE, UK
A R T I C L E I N F O Keywords: HVOF ID spray Wear WC-Co-Cr Thermal spray A B S T R A C T
Due to the restrictions and mediocre performance of current methods of coating complex shaped parts in which line of sight processes currently struggle, the development of new coating methods is essential, with High Velocity Oxy-Fuel (HVOF) thermal spray coatings being a good candidate. In this study, a new compact High Velocity Oxy-Air Fuel (HVOAF) thermal spray torch designed to coat internal surfaces was traversed within cylindrical pipes of internal diameters (IDs) of 70 mm, 90 mm and 110 mm and a WC-10Co-4Cr coating was applied with a commercially available powder feedstock. Powder and coating microstructures were analysed using SEM/EDX and XRD. Fracture toughness and microhardness of the coatings were measured, and dry sliding wear performance was investigated at two loads: 96 and 240 N. It was found that the coating sprayed at 90 mm (medium ID) had a lower speciﬁc wear rates at both test loads due to the highest fracture toughness and mi-crohardness; whereas, the coating sprayed at 110 mm (high ID) showed the highest speciﬁc wear rates at both low and high conditions due to poor fracture toughness.
The development of an alternative method of coating complex-shaped parts in which line of sight processes are limited is currently essential, due to the regulatory limitations (REACH legislation, Regulation (EC) No. 1907/2006) restricting the use of currently used methods such as electroplated hard chrome (EHC). High velocity oxy-fuel (HVOF) thermal sprayed coatings have been proposed as a good alternative to electroplated hard chrome as they are more en-vironmentally friendly, better performing and moreﬂexible in terms of the choice of coating materials available . In particular, cermet materials sprayed by HVOF such as WC-Co-Cr may be suitable to re-place EHC coatings for applications in which resistance to sliding wear is required, due to the fact that these coatings have been shown to oﬀer superior wear resistance . As a result, a number of industrial sectors such as aerospace, oﬀ-shore oil and steel production [3,4] have been searching for a way to apply thermal spray coatings on complex shaped parts traditionally processed using EHC.
The line of sight nature of thermal spray processes prevented their use in many applications, such as coating internal surfaces and complex shaped parts, due to the large dimensions and stand-oﬀ distance
required. In order to mitigate these limitations, a new generation of thermal spray systems have been developed, in the form of spray tor-ches with much smaller dimensions able toﬁt in narrower spaces an-deﬀectively coat surfaces at much shorter stand-oﬀdistances . This potentially enables the use of thermal spraying to coat internal surfaces in which non-line of sight processes like EHC were once required. However, using a spray torch with a short barrel at smaller stand-oﬀ distances produces new challenges to overcome, for instance the tem-perature of in-ﬂight particles has been shown to be strongly dependant on the length of the barrel . Consecutively, spraying at smaller stand-oﬀdistances may mean the in-ﬂight particles are still undergoing ac-celeration and heating when impacting the substrate [7,8]. Combining these two eﬀects may result in a poor coating, due to the fact the particles may have not melted suﬃciently alongside impacting the substrate at a relatively low velocity, resulting in insuﬃcient plastic deformation and low adiabatic shear instabilities . Finer powder feedstocks in particular may be more suitable than larger powders when spraying at these conditions, as smaller particles with a lower mass will accelerate at a faster rate and require less energy to reach their op-timum temperature in comparison to larger, heavier particles of the same material. Also, smaller particles have a higher surface area to
Received 26 November 2018; Received in revised form 25 April 2019; Accepted 10 July 2019
*Corresponding author. **
E-mail addresses:firstname.lastname@example.org(S. Kamnis),email@example.com(T. Hussain). Wear 432-433 (2019) 202965
Available online 11 July 2019
0043-1648/ © 2019 The Authors. Published by Elsevier B.V. This is an open access article under the CC BY license (http://creativecommons.org/licenses/BY/4.0/).
volume ratio which favours heat transfer from the hot environment. However, when spraying WC based cermet materials, it has been shown in previous work that reducing the particle size can make the WC phase more susceptible to decomposition, which for carbides is referred to as decarburisation . This eﬀect arises due to the WC grains dissolving in the molten binder phase, after which carbon will begin to be re-moved by reacting with oxygen at the gas-liquid interface . Therefore, this mechanism is strongly linked to particle temperature and, asﬁner powder particles with a lower mass require less energy to heat up in comparison to larger heavier ones, they are also more vul-nerable to overheating . Careful spray parameter optimisation and powder feedstock selection is needed to give rise to suﬃcient particle velocity to achieve a viable coating, meanwhile preventing overheating of the particles to prevent decarburisation. The coating of the surfaces inside of parts with internal diameters larger than 125 mm by HVOF ID technology has begun to be more widely accepted as the development of thisﬁeld continues. However, applying coatings using HVOF thermal spray using commercial feedstock powders within IDs less than this length, in particular IDs of 100 mm or less, has been challenging due to the previously mentioned issues. Currently little is known about the performance of HVOF coatings sprayed within cylinders with a small internal diameter; however this work presents data regarding the mi-crostructure, mechanical properties and sliding wear resistance of coatings sprayed at IDs as low as 70 mm. In this study, a compact HVOAF spray system capable of operating with a mixture of air and fuel gases developed by Castolin Eutectic-Monitor Coatings Ltd. (North Shields, UK)  was mounted within pipes with internal diameters of 70 mm, 90 mm and 110 mm and used to apply a WC-10Co-4Cr coating. The coatings microstructure and the associated mechanical properties were studied with SEM and XRD to determine the eﬀect of the changing internal diameter on each coating. Unlubricated sliding wear testing against a WC-Co counterbody was used to study the eﬀect of changing ID on the coating’s sliding wear resistance and as a means to test the performance of the three coatings. The aim of this work is to demon-strate that WC-Co-Cr HVOF thermal sprayed coatings with useful tri-bological properties can be applied on internal surfaces within cylinders of IDs as low as 70 mm, as well as showing the potential eﬀect of how changing the internal diameter aﬀects these properties in order to assist future spray parameters optimisation. Wear testing was carried out at two separate loads to simulate low and high load applications. 2. Experimental
2.1. Deposition of internally sprayed coatings
38.1 mm diameter x 6 mm discs of 416 stainless steel (12–14% Cr, 1.25% Mn, 0.15% C, 0.15% S, 0.6% Mo, 0.06% P, 1% Si in weight %) were mounted using magnets on the inside of three cylindrical tubes that, taking into account the disc and magnet thickness, correspond to spraying on cylindrical tubes with internal diameters of 70 mm, 90 mm and 110 mm. The samples obtained will be referred to with the names ID70, ID90 and ID110 throughout the text, and correspond to actual stand-oﬀ distances of 30 mm, 50 mm and 70 mm, respectively. The axial length of pipe used was 200 mm. A photograph of the setup is shown inFig. 1.
A compact HVOAF spray system developed by Monitor Coatings—Castolin Eutectic, designed to coat internal surfaces, was used to deposit the coatings. The torch uses a mixture of hydrogen (200–300 SLPM), air (100–400 SLPM) and oxygen (100–200 SLPM) depending on the mode of operation. The combustion chamber pressure was 6–8 bar. The gun was positioned inside the pipe and moved verti-cally at 2 mm/s and the substrate was rotated around it as shown in Fig. 1. In order to monitor the temperature of the part being sprayed, an external thermal imaging camera was used. To prevent overheating of the pipe the rotational speed of the part could be increased, thereby reducing the time the part is exposed to theﬂame for each pass. Air is
also blown into the cylinder to assist cooling and help the removal of undeposited particles. Fixed spray parameters were used when spraying each ID. The feedstock powder used in the study was a commercially bought powder (H. C. Starck, Munich, Germany), stated by the manu-facturer to have a particle size range of–15 + 5μm and a medium WC grain size. Details about the feedstock powder are shown inTable 1. The stainless steel discs were cleaned and grit blasted prior to coating deposition, with the spray parameters developed from previous opti-misation studies .
2.2. Dry sliding wear testing
Unlubricated sliding wear testing was carried out at room tem-perature (≈25 °C, relative humidity≈60%) using a conventional ball on disc apparatus, shown schematically in Fig. 2, following the in-structions described by the ASTMG99standard , against a 94% WC –6% Co (wt.%) ball with a diameter of 9.5 mm (Dejay Ltd, Launceston, UK) that was replaced at the end of each test. Uninterrupted wear tests with a sliding speed of 0.05 m/s and distance of 500 m were run at loads of 96 N and 240 N, with these conditions chosen with the aim of promoting wear of the coating surface and to follow on from previous work . The coeﬃcient of friction was monitored throughout the test using a LVDT (linear variable diﬀerential transformer). The top surfaces of the coatings were polished to a 1μmﬁnish and were cleaned with IMS (Industrial methylated spirit) prior to wear testing. 2 separate samples were subjected to wear testing for each coating at both loads. The volume loss of each disc was determined using the proﬁlometry method used in other studies . A surface proﬁler (Taylor Hobson Ltd, Leicester, UK) was used to measure 4 line traces perpendicular to the sliding direction to determine the cross sectional area of the wear track. These values were averaged and then multiplied by the track length to estimate the total volume of material removed during the wear test. The speciﬁc wear rate could then be calculated by dividing the total volume of material lost by the product of the load and sliding distance. The wear of the WC-Co counterbody during the test resulted in a nearﬂat surface.
The morphology of the wear scar and fracture mechanisms were then examined in plan view using a scanning electron microscope (Jeol 6490LV, Jeol Ltd., Japan), with optical microscopy (Nikon Eclipse LV100ND, Nikon, Japan) used to image the WC-Co counterbody. Cross sections of the wear scars were also imaged using SEM with secondary electrons (SE) imaging with the samples being sectioned using a SiC cutting disk and mounted in a cold mounting resin to ensure the pre-servation of important delicate features.
2.3. Coating characterisation
Coating cross sections were prepared by sectioning the sample using a SiC cutting wheel in a precision cutting saw. Powder and coating sections were then mounted in a conductive mounting compound (Metprep Ltd, UK), ground with SiC papers down to a 15.3μm grit size Fig. 1.Photograph and plan view schematic of ID coating deposition setup (drawing not to scale). The torch wasﬁxed in x and y directions and the pipe holding the substrates rotated during deposition.
and then polished down to a 1μmﬁnish. The feedstock powder, coating cross sections and wear tracks were imaged using a scanning electron microscope (Jeol 6490LV, Jeol Ltd, Japan), utilising both SE imaging and back scattered electron (BSE) imaging. X-ray diﬀraction was per-formed on the feedstock powder and coating top surfaces using a Siemens D500 with CuKαradiation (1.5406 Å) in the 20°≤2θ≤90° range to identify the phases present in the powders and coatings. A step size of 0.02° and dwell time of 3 s were used. Quantitative Rietveld reﬁnement was carried out using TOPAS (Coelho Software, Australia) to determine the phase composition within the feedstock powders and coating samples.
The microhardness of the coatings was measured on polished cross-sections by using a Vickers microhardness indenter (Buehler, Illinois, USA) at a load of 300 gf and a dwell time of 10 s; for each sample 10 indentations were made in the centre of the coatings running parallel with the substrate. Fracture toughness of the coatings was measured by indenting on polished cross sections with a 2.5 kgf load and measuring the crack lengths parallel to the substrate using optical microscopy; cracks propagating from the left and right tips of the indent were considered. The fracture toughness KIc was determined using the
method described by Evans and Wilshaw , shown in equation(1):
⎜ ⎟ = ⎛ ⎝ ⎞ ⎠ ⎛ ⎝ ⎞ ⎠ K P a a c 0.079 log 4.5 Ic 3 2 (1)
WhereP is the applied indentation load,a is the indentation half diagonal and c is the crack length from the indent centre. This ex-pression is only valid when 0.6≤c/a≤4.5; all measurements ofcanda were determined toﬁt within this range. 10 indents were measured for each coating, and the mean and standard deviation of the results is presented.
3.1. Microstructural characterisation of coatings
The XRD spectra, shown with the results of the quantitative Rietveld reﬁnement of the feedstock powder and the three sprayed coatings, are displayed inFig. 3. The phases detected in the feedstock powder consist of the primary WC phase,η-phase carbide, Co6W6C and a solid solution
of (Co,Cr). Rietveld reﬁnement was unable to give a conclusive answer on whether the (Co, Cr) solid solution found within the powder feed-stock has an fcc or hcp crystal structure, as Rietveld scores were com-parable.
All three coating spectra show that some carbon loss occurred during the spray process, as expected, due to the emergence of the W2C
phase. A right hand shoulder on the W2C peak positioned at 2θ≈40°
can be seen on all coating scans, and this can be attributed to the (422) peak of Co3W3C positioned at 2θ= 40.588° according to
PDF–01-078-5005. Using the Rietveld reﬁnement method it was determined that the W2C content of ID70 coating (6.76 wt % W2C) was slightly less than the
ID90 coating (6.81 wt % W2C). However, ID110 was found to contain a
lower weight percentage of W2C than the other two coatings, with a
calculated weight composition of 4.68%. To compensate for the lower amount of this phase in ID110, a greater weight percentage ofη-phase carbide M6C was found in this coating compared to the other two. The
diﬀraction peaks within the 2θ= 37°–46° range have been noted to have broadened slightly in comparison to the feedstock powder spec-trum. This may indicate that some amorphous material formed during the spray process due to the elevated temperatures.
SEM images of the feedstock powder and powder cross section are presented inFig. 4. The powder particles have an angular shape typical of sintered and crushed powder feedstocks with little intra particle porosity. Low and higher magniﬁcation BSE SEM images of the three coatings are shown inFig. 5. The thickness of ID70, ID90 and ID110 were measured in 4 diﬀerent locations and averaged, resulting to be (224 ± 7)μm, (214 ± 7)μm and (129 ± 4)μm respectively. Spray parameters, RPM of the part and gun vertical movement speed were kept constant when spraying all three coatings, so the actual linear speed with which the substrate is moving relative to the torch will diﬀer, possibly contributing to this thickness diﬀerence. Throughout the microstructure of all three coatings, the presence of a phase with a darker contrast is observed inFig. 5a, c and e.
An EDX point scan was undertaken on such a site (marked by the red dot onFig. 5a) and the composition was found to consist mostly of Fe, with trace amounts of Si and Mn, suggesting it originated from the 416 stainless steel substrate as no traces of these elements were found within the powder feedstock. The presence of these substrate impurities appears to be most visible within the microstructure of ID70, implying that the shorter stand-oﬀdistance required to spray the smaller internal diameter may be to blame. These Fe particles are likely to be an artefact of spraying inside a pipe where any loose debris will be attracted to the coating because of the mounting magnets.
The high magniﬁcation BSE images reveal a complex micro-structure, typical of a cermet coating. Grains of WC, appearing as the brightest phase, due to the mean atomic number in the BSE image, can be seen distributed throughout surrounded by a binder phase with a varying contrast. The varying contrast of the binder phase is an Table 1
Feedstock powder characteristics (size ranges and chemical compositions) as supplied by the manufacturer.
Powder Commercial Designation Chemical Composition (wt. %) Size range (μm)
AMPERIT®554.067 W Co Cr C O Fe D90 D10
Balance 8.5–11.5 3.0–5.0 5.0–6.0 Max 0.2 Max 0.6 18–24 5–8
Fig. 3.XRD spectra of the three sprayed coatings and feedstock powder. The blue dots represent the mea-sured data, Rietveldﬁt is shown by the red line and the blue vertical line corresponds to the maximum of split Pearson VII function that models the halo from amorphous phase(s). The quantities are shown in wt. %. The feedstock powder mainly contained WC, M12C carbides alongside a solid solution of hcp (Co,
Cr). The coatings can be seen to contain W2C and
M6C carbides. Between 2θ= 37°–46° a slight
broa-dened region can be observed on the 3 coating spectra possibly indicating amorphous material. The peak positions can be seen from the coloured marks below the scans–WC, W2C and eta carbide phase
peak positions are top, middle and bottom respec-tively. (For interpretation of the references to colour in thisﬁgure legend, the reader is referred to the Web version of this article.)
indication of tungsten dissolution into the binder phase, suggesting that particles were well melted by the torch prior to impacting the substrate. The Vickers microhardness and indentation fracture toughness of the three coatings is presented inTable 2. ID70 was found to have the lowest microhardness out of the three coatings, with the values mea-sured during these tests also having the highest standard deviation suggesting a larger degree of non-homogeneity in terms of the micro-hardness throughout this coating in comparison with the others. ID90 was found to have the highest microhardness and fracture toughness of
Fig. 4.SE SEM images of feedstock powder showing blocky, angular morphology and polished cross-section of the powder showing WC particle in a CoCr matrix.
Fig. 5.Low (left column) and high magniﬁcation (right column) BSE SE images of the three coatings with (a–b) ID70, (c–d) ID90, (e–f) ID110. An EDX spot scan was performed at the position marked onFig. 5a with the results available in the text. The WC grains (bright grey) are surrounded by a binder phase of various contrast levels (grey, black areas). Areas where WC has partially dissolved in the surrounding binder are circled.
Microhardness and indentation fracture toughness measured on the polished cross-section of three coatings. The table shows average values with standard deviation.
Sample Vickers Microhardness (300gf) Fracture toughness KIc(MPa.m0.5)
ID70 1201 ± 106 3.92 ± 0.36 ID90 1319 ± 40 4.82 ± 0.24 ID110 1310 ± 52 3.34 ± 0.52
all three coatings measured, with the standard deviation of the mea-sured values being the smallest, suggesting a more homogenous mi-crostructure. The microhardness of the ID110 coating is comparable to the harder ID90, however the fracture toughness of this coating was found to be lowest of the three coatings.
3.2. Dry sliding wear testing
The measured speciﬁc wear rates of the three coatings tested are presented inFig. 6. At 96 N ID90 shows the lowest wear, with ID110 wearing out the most. At this load, the wear of all three coatings is in the 10−7mm3/Nm range, meaning the amount of material loss is small.
At the 240 N load, ID90 again shows the lowest wear, with ID70 per-forming the worst. From analysing the relationship between the mea-sured speciﬁc wear rates of ID70 and ID90, it appears that both coatings reacted to the increase in load in a similar manner. However ID110 did not ﬁt this trend, suggesting a diﬀerent mechanism of wear may be taking place in this coating in comparison to the others.
In order to gain an understanding of the wear mechanisms taking place during the sliding wear test, the wear tracks were analysed using SEM. Images of the plan view of the wear scars formed from the 96 N tests are displayed inFig. 7. Diﬀerent magniﬁcations of the wear tracks have been used in thisﬁgure to highlight the speciﬁc features on the sample surface. On the ID70 sample, isolated areas deﬁcient of the WC hard phase are visible. This brittle phase was found in a previous study and was shown by EDX analysis to contain W = 64.7 wt%, O = 26.4 wt %, Co = 4.9%, C = 3% and Cr = 1% ; with this tungsten oxide phase probably formed by tribo-oxidation. Cracks are seen propagating across the wear track perpendicular to the direction of counterbody movement on the ID70 sample at 96 N, covering many splats at a time. At the same load, these cracks cannot be seen on the ID90 sample. The surface of the ID90 wear track is covered with micron sized pores; likely in sites where WC phase pull-out has occurred.
The wear scar of the ID110 sample at the 96 N load can be seen to have suﬀered a greater amount of material loss in comparison to the other two coatings at this load, due to many large sites of material pull-out being visible. Unlike the ID90 coating, the size of these pull-pull-out sites was found to be many times larger, with an example displayed in the high magniﬁcation image being at least 50μm in diameter. Alongside the main hole, other areas showing signs of cracks can also be observed. It should also be noted that the wear track of the ID110 sample is also much wider compared to ID90 under the same loading condition. The friction coeﬃcients for the 3 coatings at 96 N all are found to settle between 0.3 and 0.4 for ID70, and 0.5–0.6 for ID90 and ID110 after an initial breaking in period.
The wear tracks of the samples tested at 240 N are shown inFig. 8. ID70 and ID90 show similar mechanisms of wear, with visible brittle areas of the tungsten oxide observed; these oxides appear darker in the BSE images. The wear scar of the ID110 sample at 240 N was found to have cracks propagating from the edge of the track parallel to the counterbody movement direction; these then curve into the track centre at some locations. These cracks were shown to propagate in particular through the brittle binder. Such extensive cracking was only seen in ID110 coating at the higher load. It should be noted that the width of the track is relatively narrower in this sample compared to the rest under the same load. The friction coeﬃcient of the ID70 and ID90 samples at 240 N is seen to rise to a peak value between 0.7 and 0.8.
More information on the wear mechanisms taking place can be uncovered by analysing the cross section of the wear tracks by SEM, shown inFig. 9at both 96 N and 240 N. The samples were cut across the worn surface, perpendicular to the direction in which the counterbody travelled. The cross section of the ID70 and ID90 samples show a si-milar scar shape at both loads, further suggesting the same mechanism of wear is taking place when load is increased. These samples showed no evidence of sub surface cracking beneath the worn surface, sug-gesting good inter-particle bonding in these coatings. Conversely, the cross sectional SEM images of the ID110 worn surface at both loads show severe sub surface cracking, with the cracks propagating into the coating centre, roughly parallel with the substrate. Lower magniﬁcation images were chosen here to show the overall coating thickness and the nature of these cracks. The extensive damage to the coating micro-structure is in line with the volume loss measurements, the wear tracks are much deeper and the cracks propagated from the bottom of the removed material. A similar phenomenon is also observed in the ID110 coating at higher load.
The feedstock powder is found to contain WC, M12C (Co6W6C) and
hcp (Co, Cr) phases and the hcp phase could not be detected (XRD detection limit 1–2 wt%) in all three coatings. The XRD spectra reveal that the W2C is present in all three coatings but not in the powder
feedstock, indicating that some carbon loss is occurring during spraying and that particle temperatures were suﬃcient to allow some degree of binder phase melting. The presence of peak broadening in the region 2θ= 37°–46° on all coating spectra have been shown by others to possibly indicate the presence of amorphous or nanostructured material . It is interesting to note that in all three coatings M6C (Co3W3C)
carbide was detected instead of M12C, which was present in the original
powder feedstock. Rietveld reﬁnement uncovered some diﬀerences in Fig. 6.Speciﬁc wear rates of the three coatings at 96 N and 240 N with error bars showing the total range of values measured.
the phase composition of the three coatings; ID110 was found to have a lower weight percentage of W2C (4.68 wt%) and greater amounts of
M6C (8.19 wt%) in comparison to the other two coatings. The formation
ofηphase carbides has been shown to occur when a carbon deﬁciency exists at the hard phase–binder interface , suggesting that more carbon was oxidised out of the equilibrium melt duringﬂight due to the greater stand-oﬀdistance leading to a greater M6C composition in the
ID110 coating. The greater weight composition of M6C carbides found
in ID110 in comparison to the other coatings may explain why this coating was found to have the lowest fracture toughness of the three coatings, as it has been shown that the increased presence of this phase worsens the mechanical properties of the material .
The speciﬁc wear rates of the three coatings and images of the wear tracks inFigs. 6–9indicate that two diﬀerent mechanisms of wear are occurring in the ID70/ID90 and ID110 coatings.
The ID70 96 N wear scar is characterised by cracks seen protruding along the entire width of the scar, accompanied by evidence of oxidised material. At the higher load, this oxidised material is visible in large amounts. A possible mechanism to explain what is occurring is as fol-lows: due to the lower microhardness of the ID70 coating, material can more readily be broken oﬀ the surface when in contact with the counterbody. This debris is then oxidised due to the heat generated between the worn surface and counterbody and this oxidised material then remains in contact with the counterbody until it falls into the holes in the worn surface. As the load is increased, the eﬀect is ampliﬁed due
to the greater contact pressure leading to accelerated debris formation, heat generation and therefore oxidation. As the size of these oxidised sites is roughly in the range of that of one of more feedstock particles, it is likely the coating is breaking on a multi splat level. This may indicate a possible cohesion issue in this coating, meaning that delamination of individual or groups of splats is more easily induced when under load. Due to the short stand-oﬀdistance, it is likely that particles are still undergoing acceleration prior to impacting the substrate; this may ex-plain why these issues are seen in the ID70 coating and not the other two.
At 96 N the main mechanism of wear for the ID90 sample appears to occur due the pull-out of the WC phase, as seen by other researchers . The perimeter of the remaining holes are smooth edges of binder phase, characteristic of a brittle fracture. This suggests that for this sample the mechanism of wear was possibly dominated by brittle fracture of the binder. When the load was increased to 240 N, regions with larger areas of material pull-out can be observed. The existence of these areas could be due to the coalescing of cracks propagating through the brittle binder, greatly reducing the material toughness in these regions.
Alongside these regions, areas of the same brittle tribo-oxidation observed on the ID70 sample can be seen.
The friction coeﬃcient of ID70 and ID90 was seen to increase to a peak value of almost 0.8; this did not happen in the other tests. These periods of increased friction coeﬃcient may explain the increased Fig. 7.Plan view SEM SE images of the wear scars produced from the sliding wear tests at 96 N. The position of the wear track lies between the arrows. The images on the right show higher magniﬁcation BSE images of the wear track surface, with an area in which WC grain pull-out has occurred circled.
oxidised debris, as more energy will be converted into heat during these periods, increasing the oxidation rate of debris. As oxidised material was not found on the worn surfaces where this friction coeﬃcient in-crease did not occur, then it is likely this may be the cause.
A smaller increase in speciﬁc wear rate was measured for ID110 when the load was raised from 96 N to 240 N, and SEM images of the wear tracks of this sample show the smallest diﬀerence in track width between the two loads. Parabolic shaped cracking is observed at the 240 N load, with the cracks propagating from within the track per-pendicular to the counterbody movement to outside the track, parallel to the movement of the counterbody. This failure mode is characteristic of a buckling mechanism, in which the failure occurs due to the ma-terial’s response to the compressive stresses generated ahead of the counterbody. Cracks are formed at the edge of the wear track due to the counterbody pushing the coating material outwards towards the edge of the track. Localised regions of the coating with interfacial defects pro-vide areas in which the coating is allowed to buckle in response to these stresses , and these buckles can then spread by propagation of in-terfacial cracks. The high magniﬁcation SEM image in Fig. 8 shows crack propagation occurs preferentially around areas high in the WC phase, highlighting these areas as potential weak points. Although the speciﬁc wear rate of this coating at 240 N was found to be lower than that of the ID70, the way this coating has worn in response to these wear tests suggests that this coating may not currently be suitable for
any practical application at higher loads.
Overall, ID70 performed worse than ID90 across both loads due to the increased microhardness and fracture toughness of the ID90 coating. ID110 was found to crack at both loads unlike the other coatings, due to having a reduced fracture toughness. From the results of this study, it appears that the fracture toughness of the coatings has a more dominant eﬀect on the sliding wear resistance in comparison to microhardness, in particular at the 96 N load. This conclusion can be made due to the fact that while the microhardness of ID90 and ID110 was found to be very similar, the mechanism of wear and speciﬁc wear rate was very diﬀerent. Visual evidence from the SEM images inFigs. 7 and 8show that brittle fracture of the binder phase is the main cause of wear, regardless of whether individual WC grain pull-out or larger scale material pull-out is occurring. The lower fracture toughness of the ID110 resulted in increased crack propagation from the wear tests, in comparison to the other two samples, leading to the highest measured speciﬁc wear rate at 96 N. Meanwhile when increasing the load to 240 N the ID70 coating then suﬀered the most wear. This coating had the lowest microhardness of the three coatings, suggesting that at the high load the microhardness of the coating starts to become key.
The mechanical properties of the sprayed coatings and results from the dry sliding wear testing suggest that the most durable coating for a wear resistance application was ID90, suggesting that when using the selected spray parameters, spraying within an internal diameter of Fig. 8.Plan view SEM images of the wear scars produced from the sliding wear tests at 240 N for all three coatings. The images on the left column show low magniﬁcation SE images of the wear track and the image on the right column show higher magniﬁcation BSE images of the track. Areas in which brittle coating material has broken oﬀhave been marked with an arrow.
90 mm provides the optimum stand-oﬀdistance of 50 mm. The ID70 coating was found to have the lowest microhardness and this may be due to the fact that when spraying at stand-oﬀdistances this small, particles are still undergoing acceleration and heating. The micro-hardness of WC-Co-Cr coatings has been shown to be inﬂuenced heavily by inﬂight particle properties, with slower particle velocities and lower temperatures often resulting in softer coatings [21,22]. At the other end of the scale, ID110 was found to have higher microhardness, but its fracture toughness was reduced in comparison to the other coatings. At higher stand-oﬀdistances, particles have a longer time to react with atmospheric gases at elevated temperature, leading to greater amounts of brittle η-carbides in the microstructure and overall lower fracture toughness.
For comparison, a similar WC-CoCr coating sprayed using com-mercially used parameters using a MetJet IV spray torch (Metallisation Ltd, UK) was subjected to dry sliding wear testing against a WC-Co counterbody using the same parameters as those used in this study at 96 N, and the sliding wear rate was determined to be 1.42 × 10−8
mm3/Nm. This comparison suggests that the internally sprayed coat-ings will perhaps require further optimisation; nonetheless, the coatcoat-ings presented here show excellent wear performance for small ID cylinders that are relevant to many high value engineering applications.
Three WC-10Co-4Cr coatings were sprayed using a compact HVOAF
spray torch developed by Castolin-Eutectic Monitor Coatings Ltd, (UK) in a setup allowing for the simulation of coating the internal surface of a cylindrical pipe with internal diameter of 70 mm, 90 mm and 110 mm. The microstructure of the powders and coatings was analysed by SEM imaging and XRD analysis with Rietveld Reﬁnement, with the me-chanical properties and resistance to dry sliding wear measured as a performance metric.
The ID90 coating was found to possess the best mechanical prop-erties of all coatings tested and, as a result, performed the best in the wear testing both at 96 N and at 240 N loads. The coating sprayed within the 70 mm ID was shown to perform better than the 110 mm ID at 96 N in the wear tests. However, further increasing the pipe internal diameter to 110 mm resulted in reduced fracture toughness of the coating and higher wear rate at both loads. This conﬁrms that, when using the spray parameters utilised in this study, a stand-oﬀdistance of 50 mm, appears to provide the optimum to obtain the best mechanical and wear performance. Particles sprayed at the lower stand-oﬀdistance may not reach the optimal velocity for impact, meanwhile those sprayed in the larger sized ID were exposed to high temperatures for a longer period, leading to a more brittle coating.
The results in this paper indicate that WC-Co-Cr powder from a commercial feedstock can be deposited on internal surfaces by the HVOF process, producing a coating without large defects. However it has been shown that using the same spray parameters when spraying all three diﬀerent IDs may not be optimal, as the mechanical properties of the coating were worse for the ID70 and ID110 coatings, which was Fig. 9.SE SEM images showing the cross section of the wear scars produced from sliding wear testing at 96 N and 240 N.
seen to aﬀect the tribological performance. Wear rate at 96 N was seen to be largely aﬀected by the fracture toughness of the coatings, with the most brittle sample (ID110) expressing the highest wear. When load was increased to 240 N, the sample sprayed at the shortest stand-oﬀ distance was found to wear the most due to its low microhardness. Speciﬁc parameter optimisation when spraying each separate ID may be required to improve the mechanical properties and therefore the wear resistance for each coating in order to further improve their tri-bological performance.
This work was supported by the Engineering and Physical Sciences Research Council [EP/L016362/1]; in the form of an EngD studentship and industrial funding from Castolin Eutectic- Monitor Coatings Ltd. References
 J. Picas, M. Punset, M. Teresa Baile, E. Martín, A. Forn, Tribological evaluation of HVOF thermal-spray coatings as a hard chrome replacement, Surf. Interface Anal. 43 (10) (2010) 1346–1353.
 T. Gong, P. Yao, X. Zuo, Z. Zhang, Y. Xiao, L. Zhao, et al., Inﬂuence of WC carbide particle size on the microstructure and abrasive wear behavior of WC–10Co–4Cr coatings for aircraft landing gear, Wear 362–363 (2016) 135–145.
 P. Fauchais, J. Heberlein, M. Boulos, Thermal Spray Fundamentals from Powder to Part, Springer, New York, 2014.
 B. Allcock, P. Lavin, Novel composite coating technology in primary and conversion industry applications, Surf. Coat. Technol. 163–164 (2003) 62–66.
 C. Lyphout, S. Bjorklund, Internal diameter HVAF spraying for wear and corrosion applications, J. Therm. Spray Technol. 24 (2015) 235–243.
 L. Zhao, M. Maurer, F. Fischer, R. Dicks, E. Lugscheider, Inﬂuence of spray para-meters on the particle in-ﬂight properties and the properties of HVOF coating of WC-CoCr, Wear 257 (1–2) (2004) 41–46.
 W. Lih, S. Yang, C. Su, S. Huang, I. Hsu, M. Leu, Eﬀects of process parameters on molten particle speed and surface temperature and the properties of HVOF CrC/
NiCr coatings, Surf. Coat. Technol. 133–134 (2000) 54–60.
 V. Katranidis, S. Gu, B. Allcock, S. Kamnis, Experimental study of high velocity oxy-fuel sprayed WC-17Co coatings applied on complex geometries. Part A: inﬂuence of kinematic spray parameters on thickness, porosity, residual stresses and micro-hardness, Surf. Coat. Technol. 311 (2017) 206–215.
 S. Gu, S. Kamnis, Bonding mechanism from the impact of thermally sprayed solid particles, Metall. Mater. Trans. A 40 (11) (2009) 2664–2674.
 J. Pulsford, S. Kamnis, J. Murray, M. Bai, T. Hussain, Eﬀect of particle and carbide grain sizes on a HVOAF WC-Co-Cr coating for the future application on internal surfaces: microstructure and wear, J. Therm. Spray Technol. 27 (1–2) (2017) 207–219.
 B. Kear, G. Skandan, R. Sadangi, Factors controlling decarburization in HVOF sprayed nano-WC/Co hardcoatings, Scr. Mater. 44 (8–9) (2001) 1703–1707.  S. Gu, S. Kamnis, Numerical modelling of in-ﬂight particle dynamics of
non-sphe-rical powder, Surf. Coat. Technol. 203 (22) (2009) 3485–3490.
 B. Allcock, S. Gu, S. Kamnis, Nozzle for a Thermal Spray Gun and Method of Thermal Spraying, (2013), p. EP2411554A.
 ASTM G99-17, Standard Test Method for Wear Testing with a Pin-on-Disk Apparatus, ASTM International, West Conshohocken, PA, 2017.
 A.G. Evans, T.R. Wilshaw, Quasi-static solid particle damage in brittle solids—I. Observations analysis and implications, Acta Metall. 24 (10) (1976) 939–956.  C. Verdon, A. Karimi, J. Martin, A study of high velocity oxy-fuel thermally sprayed
tungsten carbide based coatings. Part 1: Microstructures, Mater. Sci. Eng. A 246 (1–2) (1998) 11–24.
 L.M. Berger, P. Ettmayer, P. Vuoristo, T. Mäntylä, W. Kunert, Microstructure and properties of WC-10%Co-4% Cr spray powders and coatings: Part 1. Powder char-acterization, J. Therm. Spray Technol. 10 (2) (2001) 311–325.
 G. Lee, S. Kang, Sintering of nano-sized WC–Co powders produced by a gas re-duction–carburization process, J. Alloy. Comp. 419 (1–2) (2006) 281–289.  T. Sudaprasert, P. Shipway, D. McCartney, Sliding wear behaviour of HVOF sprayed
WC–Co coatings deposited with both gas-fuelled and liquid-fuelled systems, Wear 255 (7–12) (2003) 943–949.
 S. Bull, Failure mode maps in the thinﬁlm scratch adhesion test, Tribol. Int. 30 (7) (1997) 491–498.
 X. Guo, M. Planche, J. Chen, H. Liao, Relationships between in-ﬂight particle characteristics and properties of HVOF sprayed WC-CoCr coatings, J. Mater. Process. Technol. 214 (2) (2014) 456–461.
 J.A. Picas, M. Punset, M.T. Baile, E. Martín, A. Forn, Eﬀect of oxygen/fuel ratio on the in-ﬂight particle parameters and properties of HVOF WC-CoCr coatings, Surf. Coat. Technol. 205 (2011) S364–S368.